Warm Tip: If you want to know more information, like quotation, products, solutions, etc., please Click here ,and contact us online.
Gold cyanide leaching process is the main method for extracting gold from ores or concentrates by using cyanide. But do you know the factors affecting gold cyanide leaching process?
In the mineral processing tests for gold cyanide leaching, it usually selects variables to test, such as grinding fineness, cyanide dosage, pulp density, leaching time, inflating volume and the temperature, pH, and agitating speed of pulp. The above variables are the major factors affecting gold cyanide leaching. Then, we will specifically explore the impact of the above factors on gold cyanide leaching.
Generally speaking, the determination of grinding fineness is related to the ore characteristics. The grinding fineness is affected by the different ore characteristics, the size and form of gold particles. After carrying out tests on the -0.074mm content of 70%, 75%, 80%, 85% and 90% respectively, the mineral processing test personnel found that:
● When the part of -0.074mm accounted for 85%, the recovery rate of gold is better.
● When one-stage grinding fineness was increased from 70% to 85%, the leaching rate of gold was increased from 82%-85% to 91.0%.
For different gold ores, the grinding fineness should be determined through mineral processing test, and it has a direct influence on the final recovery rate of gold ores.
Gold is a kind of inactive metal, which can cause complexation reaction with cyanogen (CN-) under the action of oxygen in the gold cyanide leaching process, and then results in Au (CN) 2-. Therefore, cyanide agent dosage is one of the key factors determining the gold leaching.
In general, the pulp should contain a certain amount of unbonded cyanogen, then the gold cyanide leaching can keep normal. And the specific dosage of cyanide agent should be determined according to the property of gold ore.
Pulp density refers to the solid-liquid ratio of pulp, which can directly affect the diffusion rate of components, and then affect the gold leaching rate and speed. It is suggested to determine the appropriate pulp density through the mineral processing test.
● When the pulp density is too high, the pulp is difficult to flow and the gold leaching speed and rate is decreased.
● When the pulp density is too low, the gold leaching speed and rate are improved, but the requirements on equipment volume are increased. So, the equipment investment cost is significantly increased, and the amount of cyanide agent will be increased correspondingly.
Gold cyanide leaching is a relatively slow process, the leaching time is over 24 hours generally, and the gold leaching rate is improved with the extension of leaching time, but the gold leaching speed is reduced corresponding, and finally the gold leaching rate tends to a limit value. At that time, even the leaching time is extended, the gold leaching rate of is not improved obviously.
Taking a low-grade oxidized gold ore containing carbon and arsenic as an example, the leaching test was carried out when the grinding fineness -0.074mm accounted for 95%, the pulp density was 33% and pH value was 12, the gold leaching rate kept 81.48% when the leaching time was 24 hours, 36 hours and 48 hours respectively.
For gold leaching, the leaching time should be determined according to the results of the mineral processing test. Blindly extend the leaching time cannot greatly improve the gold leaching rate.
The reason for gold leaching needs to be inflated is that effective oxidation is conducive to the gold dissolution, so appropriately inflating can improve the solubility of oxygen in pulp, thus improving the dissolution rate of gold. Usually, increasing the inflating volume can be finished by inflating or agitating the pulp.
The reason why the temperature, pH, and agitating speed of pulp affect gold leaching is that cyanide is easy to generate hydrocyanic acid (HCN) through reaction in the pulp. Hydrocyanic acid is volatile and toxic. If hydrocyanic acid volatiles from the pulp, it will cause cyanide loss and environmental pollution.
Therefore, in the gold cyanide leaching process, the pulp temperature maintains an appropriate value (usually less than 15 ℃) and the pH value of the pulp is generally adjusted to 10-11, and keeping uniform agitating, which can prevent the volatilization of hydrocyanic acid.
In conclusion, we can change the above factors to improve the gold leaching rate in cyanide leaching process for refractory gold ores. It is suggested that the mineral owners should entrust a qualified mineral processing testing institution to conduct the mineral processing test, and determine the appropriate gold leaching reagents through the mineral processing test results, so that the mineral processing plant can obtain the reasonable process indicators, and avoid the late recovery after the production, reduce the loss of the mineral processing plant.
No. 188, Xinhai Street, high-tech Industrial Park, Fushan District, Yantai, Shandong, China.